Selenate selenite

Short description: Class of chemical compounds

A selenate selenite is a chemical compound or salt that contains selenite and selenate anions (SeO32- and SeO42-). These are mixed anion compounds. Some have third anions.

## Contents

* 1 Naming
* 2 Production
* 3 Properties
* 4 Related
* 5 List
* 6 References

## Naming

A selenate selenite compound may also be called a selenite selenate.

## Production

One way to produce a selenate selenite compound is to evaporate a water solution of selenate and selenite compounds.[1]

## Properties

On heating, selenate selenites lose SeO2 and O2 and yield selenites, and ultimately metal oxides.[2]

## Related

Related to these are the sulfate sulfites and tellurate tellurites. They can be classed as mixed valent compounds.

## List

name  | formula  | ratio

SeO4:SeO3

| mw | system  | space group | unit cell Å  | volume  | density  | properties  | references

|
|
|
|
|
|
|
|
|
|

Boroseleniteselenate  | B2Se3O10 | 1:2  |  | monoclinic  | P21/c | a = 4.3466, b = 7.0237, c = 22.1460, β = 94.922°, Z = 4  |  |  | colourless hygroscopic  | [3]
| Na2(SeO4)(H2SeO3)· H2O  | 1:1  |  | orthorhombic  | Cmc21 | a=9.615, b=11.19, c=9.62 Z=4  |  |  |  | [4]
| Sc2(SeO3)2(SeO4)  | 1:2  |  | monoclinic  | P21/c | a = 6.5294, b = 10.8557, c = 12.6281, β = 103.543° Z = 4  | 870.21  |  |  | [5]
| Sc2(TeO3)(SeO3)(SeO4)  | 1:1  |  | monoclinic  | P21/c | a = 6.535, b = 10.970, c = 12.559, β = 102.70° Z = 4  | 878.3  |  |  | [5]
| Fe(SeO4)(HSeO3)· H2O  | 1:1  |  | monoclinic  | P21/c | a=8.355,b=8.696,c=9.255, β=93.72°,Z=4  | 670.95  |  |  | [6]
Lithium sequicopper selenite selenate  | Li2Cu3(SeO3)2(SeO4)2 | 2:2  |  | monoclinic  | I2/a | a=16.293,b=5.007,c=14.448, β = 94.21°, Z=4  | 1175.5  |  |  | [7]
| RbFe(SeO3)(SeO4)  | 1:1  |  |  |  | a=5.339, c=41.206, Z=6  | 1040.2  |  |  | [8]
| Y2(SeO3)2(SeO4)(H2O)2·(H2O)0.75 | 1:2  |  | monoclinic  | C2/c | a=11.9118 b=6.8886 c=12.9644 β=103.839°  |  |  | UV cut off 211 nm  |
| Zr(SeO3)(SeO4)  | 1:1  |  | orthorhombic  | Pbca | a = 8.291, b = 9.458, c = 15.357, Z = 8  | 1204.2  |  |  | [9]
| Zr4(SeO3)(SeO4)7 | 7:1  |  | monoclinic  | P21/n | a = 5.313, b = 10.704, c = 10.484, β = 104.13°, Z = 1  | 578.2  |  |  | [9]
| Zr3(SeO3)(SeO4)5·2H2O  | 5:1  |  | triclinic  | P1  | a = 5.273, b = 8.079, c = 11.959, α = 82.60°, β = 88.27°, γ = 89.87°, Z = 1  | 505.1  |  |  | [9]
| Ag4(Mo2O5)(SeO4)2(SeO3)  | 2:1  |  | orthorhombic  | Pbcm | a=5.6557, b=15.8904, c=15.7938, Z=4  | 1419.4  |  |  | [10]
tricadmium(II) bis-[selenite(IV)] selenate(VI)  | Cd3(SeO3)2(SeO4)  | 1:2  |  | monoclinic  | P21 | a=8.302 b=5.337 c=10.843 β =108.641 Z=2  | 876.32  | 4.539  | SHG 0.6×KDP; stable to 482 °C  | [2]
| (NH4)4Cd(HSeIVO3)2(SeVIO4)2 | 2:2  |  | triclinic  | P1 | a = 5.791 b = 7.411 c = 10.736 α = 90.05° β = 105.02° γ = 112.61°  | 408.2  |  |  | [11]
| Ag2Cd(Se2O5)(Se0.3S0.7O4)  |  | 676.19  | triclinic  | P1 | a=6.7485 b=6.8504 c=9.769 α=101.36° β=105.96° γ=91.159° Z=2  | 424.41  | 5.291  | yellow  | [12]
| Sb2(SeO3)2SeO4 | 1:2  | 640.38  | monoclinic  | I2/a | a=8.1184 b=7.4572 c=14.7625 β=94.892° Z=4  | 890.47  | 4.777  | birefringence 0.158 @ 546  | [13]
| La2(HSeO3)(SeO4)· 2H2O  | 1:1  |  | monoclinic  | P21/n  | a=7.272 b=9.409 c=11.940 β =93.32°  |  |  |  | [1]
| NaLa(SeO3)(SeO4)  | 1:1  |  | monoclinic  | P21/c | a=10.751 b=7.098 c=8.437 β =90.90°  |  |  |  | [1]
| Pr4(SeO3)2(SeO4)F6 | 1:2  |  | monoclinic  | C2/c | a = 22.305, b = 7.1054, c = 8.356, β = 98.05°, Z = 4  |  |  | light green  | [14]
dineodymium diseleite selenate  | Nd2(SeO3)2(SeO4) · 2H2O  | 1:2  | 721.39  | monoclinic  | C2/c | a = 12.276, b = 7.0783, c = 13.329, β = 104.276°  | 1122.4  | 4.27  | pink  | [15]
| NaSm(SeO3)(SeO4)  | 1:1  |  | monoclinic  | P21/c | a = 10.669, b = 6.9166, c = 8.2588, β = 91.00° Z = 4  |  |  | light yellow  | [1]
| Er2(SeO3)2(SeO4) · 2H2O  | 1:2  |  | monoclinic  | C2  | a=11.935 b=6.881 c=6.473 β =103.79° Z=4  |  |  |  | [1][16]
| Hf(SeO3)(SeO4)(H2O)4 | 1:1  |  | orthorhombic  |  |  |  |  |  | [17]
| Au2(SeO3)2(SeO4)  | 1:2  |  | orthorhombic  | Cmc21 | a = 16.891, b = 6.3013, c = 8.327, Z = 4  | 886.2  |  | orange yellow  | [18]
| Hg2(SeO3)(SO4)  | 1:1  | 624.20  | monoclinic  |  | a=6.3799 b=7.0185 c=13.4426 β=94.511° Z=4  | 600.06  | 6.909  | birefringence 0.133@532 nm and 0.126@1064 nm  | [19]
| Hg3(SeO3)2(SeO4)  | 1:2  |  | monoclinic  | P21 | a = 8.3979 b = 5.3327 c = 11.148 β = 108.422° Z = 2  | 473.67  |  | colourless  | [20]
| Hg3Se(SeO3)(SO4)  |  |  | monoclinic  | P21/n | a=7.1188 b=9.9209 c=12.4565 β=95.398° Z=4  | 875.84  | 6.854  | colourless; band gap 3.5 eV; birefringence 0.069@546 nm  | [21]
| Hg5O(SeO3)(SeO4)  | 1:1  | 1288.87  |  | C2/c | a=17.563 b=6.188 c=18.912 β =90.379 Z=8  | 2055.2  | 8.331  | yellow  | [22]
| Hg3Hg2Hg(HgO2)(SeO3)2(SeO4)·H2O  | 1:2  |  |  | R3  | a=5.9239 c=37.096 Z=3  |  |  |  | [23]
| Hg3Hg2Hg2(HgO2)(SeO3)2(SeO4)2·H2O  | 2:1  |  |  | P31c | a=5.8908 c=31.048 Z=2  |  |  |  | [23]
| Ag4Hg(SeO3)2(SeO4)  | 1:2  | 1028.95  | orthorhombic  | Cmc21 | a=8.1690 b=11.9903 c=10.8870 Z=4  | 1066.4  | 6.409  | 398 nm cutoff NLO 0.35×KDP  | [24]
| La2Hg3(SeO3)4(SO4)2(H2O)2 | 4:2  | 1611.55  | triclinic  |  | a=9.1127 b=9.2446 c=13.5562 α=86.099 β=79.267 γ=61.814 Z=2  | 988.73  | 5.413  |  | [12]
| Pb2(SeO3) (SeO4)  | 1:1  | 684.30  | orthorhombic  | Pnma | a=13.5080 b=5.6238 c=9.2706 Z=4  | 704.25  | 6.454  | stable to 232 °C  | [2]
schmiederite  | Pb2Cu2(OH)4(SeO3)(SeO4)  | 1:1  |  | monoclinic  | P21/m | a = 9.922, b = 5.712, c = 9.396, β = 101.96°, Z = 2  |  |  |  | [25]
| Bi2(SeO3)2(SeO4)  | 1:2  | 814.84  | monoclinic  | I2/a | a= 8.0440 b=7.4377 c=14.7456 β =97.274 Z=4  | 875.11  | 6.184  | colourless  | [26]
| Ag2Bi2(SeO3)3(SeO4)  | 1:3  | 1157.54  | monoclinic  | P21/m | a=9.5380 b=5.4965 c=11.8207 β =92.892 Z=2  | 618.92  | 6.211  | 339 nm cutoff  | [24]
| Th(SeO3)(SeO4)  | 1:1  |  | monoclinic  | P21/c | a=7.0351 b=9.5259 c=9.02266 β =103.128, Z=4  |  |  |  | [27]
| (H3O)[(UO2)(SeO4)(SeO2OH)]  | 1:1  |  | monoclinic  | P21/n | a = 8.668, b = 10.655, c = 9.846, β = 97.88°  | 900.7  |  |  | [28]
| [C5H14N][(UO2)(SeO4)(SeO2OH)]  | 1:1  |  | monoclinic  | P21/n | a=11.553, b=10.645, c=12.138, β=108.05, Z=4  |  |  |  | [29]
| [C5H14N]4[(UO2)3(SeO4)4(HSeO3)(H2O)]·(H2SeO3)(HSeO4)  | 5:2  |  | triclinic  | P1 | a = 11.7068, b = 14.816, c = 16.977, α = 73.899°, β = 76.221°, γ = 89.361°, Z = 2  | 2743.0  |  |  | [30]
catena-(bis(Dimethylammonium) oxonium tetrakis(μ3-selenato)-(μ2-selenito)-aqua-hexaoxo-tri-uranium selenous acid)  | [C2H8N]2[H3O][(UO2)3(SeO4)4(HSeO3)(H2O)](H2SeO3)0.2 | 4:1.2  |  | monoclinic  | P21/m | a 8.3116 b 18.6363 c 11.5623 β =97.582°  |  |  |  | [31]
catena-(tris(Dimethylammonium) tetrakis(μ3-selenato)-(μ2-hydrogen selenito)-aqua-hexaoxo-tri-uranium dimethylamine)  | [C2H8N]3(C2H7N)[(UO2)3(SeO4)4(HSeO3)(H2O)]  | 4:1  |  | orthorhombic  | Pnma | a =11.659 b =14.956 c =22.194  |  |  |  | [31]
| [NH3(CH2)9NH3][(UO2)(SeO4)(SeO2OH)](NO3)  | 1:1  |  | triclinic  | P1 | a = 10.7480, b = 13.8847, c = 14.636, α = 109.960°, β = 103.212°, γ = 90.409°, Z= 4  | 1990.0  |  |  | [32]
| Cs2(H2O)5[(UO2)7(SeO4)2(SeO3)2O4]. H2O  | 2:2  |  | monoclinic  | P21/m  | a =.1381, b =15.0098, c =15.1732 β=91.17°  |  |  |  | [33]

## References

1. ↑ 1.0 1.1 1.2 1.3 1.4 Wickleder, Mathias S. (June 2002). "Inorganic Lanthanide Compounds with Complex Anions" (in en). Chemical Reviews 102 (6): 2057–2062. doi:10.1021/cr010308o. ISSN 0009-2665. PMID 12059261. https://pubs.acs.org/doi/10.1021/cr010308o.
2. ↑ 2.0 2.1 2.2 Shang, Meng; Halasyamani, P. Shiv (June 2020). "Mixed-valent selenium compounds: Noncentrosymmetric Cd3(SeO3)2(SeO4) and Hg3(SeO3)2(SeO4) and centrosymmetric Pb2(SeO3) (SeO4)" (in en). Journal of Solid State Chemistry 286. doi:10.1016/j.jssc.2020.121292. Bibcode: 2020JSSCh.28621292S. https://linkinghub.elsevier.com/retrieve/pii/S0022459620301225.
3. ↑ Daub, Michael; Scherer, Harald; Hillebrecht, Harald (2015-03-02). "Synthesis, Crystal Structure, and Spectroscopy of the Mixed-Valent Boroseleniteselenate B 2 Se 3 O 10" (in en). Inorganic Chemistry 54 (5): 2325–2330. doi:10.1021/ic502916j. ISSN 0020-1669. PMID 25695146. https://pubs.acs.org/doi/10.1021/ic502916j.
4. ↑ Baran, J.; Lis, T.; Marchewka, M.; Ratajczak, H. (October 1991). "Structure and polarized IR and Raman spectra of Na2SeO4·H2SeO3·H2O crystal" (in en). Journal of Molecular Structure 250 (1): 13–45. doi:10.1016/0022-2860(91)80119-O. Bibcode: 1991JMoSt.250...13B. https://linkinghub.elsevier.com/retrieve/pii/002228609180119O.
5. ↑ 5.0 5.1 Song, Seung Yoon; Lee, Dong Woo; Ok, Kang Min (2014-07-07). "Rich Structural Chemistry in Scandium Selenium/Tellurium Oxides: Mixed-Valent Selenite–Selenates, Sc2(SeO3)2(SeO4) and Sc2(TeO3)(SeO3)(SeO4), and Ternary Tellurite, Sc2(TeO3)3" (in en). Inorganic Chemistry 53 (13): 7040–7046. doi:10.1021/ic501009c. ISSN 0020-1669. PMID 24918773. https://pubs.acs.org/doi/10.1021/ic501009c.
6. ↑ Giester, Gerald (November 1992). "The crystal structure of Fe(SeO2OH)(SeO4)·H2O" (in en). Monatshefte für Chemie 123 (11): 957–963. doi:10.1007/BF00810925. ISSN 0026-9247. http://link.springer.com/10.1007/BF00810925.
7. ↑ Giester, Gerald (1989). "Crystal structure of Li2Cu3(SeO3)2(SeO4)2" (in en). Monatshefte für Chemie 120 (8–9): 661–666. doi:10.1007/BF00809956. ISSN 0026-9247. http://link.springer.com/10.1007/BF00809956.
8. ↑ Giester, Gerald (August 2000). "Syntheses and crystal structures of the new compounds BaFe2(SeO3)4, AgFe(SeO3)2 and RbFe(SeO4)(SeO3)" (in en). Journal of Alloys and Compounds 308 (1–2): 71–76. doi:10.1016/S0925-8388(00)00848-3. https://linkinghub.elsevier.com/retrieve/pii/S0925838800008483.
9. ↑ 9.0 9.1 9.2 Wildner, Manfred; Giester, Gerald (April 2019). "Contributions to the stereochemistry of zirconium oxysalts—part II: syntheses and crystal structures of Zr(SeO3)(SeO4), Zr4(SeO3)(SeO4)7, and Zr3(SeO3)(SeO4)5·2H2O" (in en). Monatshefte für Chemie 150 (4): 593–603. doi:10.1007/s00706-019-2352-x. ISSN 0026-9247. http://link.springer.com/10.1007/s00706-019-2352-x.
10. ↑ Ling, Jie; Albrecht-Schmitt, Thomas E. (May 2007). "Syntheses, structures, and properties of Ag4(Mo2O5)(SeO4)2(SeO3) and Ag2(MoO3)3SeO3" (in en). Journal of Solid State Chemistry 180 (5): 1601–1607. doi:10.1016/j.jssc.2007.02.020. Bibcode: 2007JSSCh.180.1601L. https://linkinghub.elsevier.com/retrieve/pii/S0022459607000941.
11. ↑ Kolitsch, Uwe (2004-01-15). "(NH4)4Cd(HSeIVO3)2(SeVIO4)2: a new structure type with kröhnkite-like chains". Acta Crystallographica Section C Crystal Structure Communications 60 (1): i3–i6. doi:10.1107/S0108270103026040. ISSN 0108-2701. PMID 14712015. Bibcode: 2004AcCrC..60I...3K. http://scripts.iucr.org/cgi-bin/paper?S0108270103026040.
12. ↑ 12.0 12.1 Li, Peng-Fei; Hu, Chun-Li; Kong, Fang; Mao, Jiang-Gao (2022). "Hg 2 (SeO 3 )(SO 4 ): the first sulfate selenite with large birefringence explored from d 10 transition metal compounds" (in en). Materials Chemistry Frontiers 6 (23): 3567–3576. doi:10.1039/D2QM00773H. ISSN 2052-1537. https://xlink.rsc.org/?DOI=D2QM00773H.
13. ↑ Luo, Han; Chen, Siyu; Li, Bailiang; Cao, Liling; Dong, Xuehua; Huang, Ling; Zou, Guohong (2026-01-07). "Sb 2 (SeO 3 ) 2 SeO 4 : A Selenite–Selenate Crystal with Balanced Band Gap and Birefringence" (in en). Crystal Growth & Design 26 (1): 582–588. doi:10.1021/acs.cgd.5c01465. ISSN 1528-7483. https://pubs.acs.org/doi/10.1021/acs.cgd.5c01465.
14. ↑ Krügermann, Ina; Wickleder, Mathias S. (2002). "Pr4(SeO3)2(SeO4)F6 und NaSm(SeO3)(SeO4): Selenit-Selenate der Selten-Erd-Elemente" (in de). Zeitschrift für anorganische und allgemeine Chemie 628 (1): 147–151. doi:10.1002/1521-3749(200201)628:1<147::AID-ZAAC147>3.0.CO;2-8. ISSN 1521-3749. https://onlinelibrary.wiley.com/doi/abs/10.1002/1521-3749(200201)628:1<147::AID-ZAAC147>3.0.CO;2-8.
15. ↑ Berdonosov, P. S.; Schmidt, P.; Dityat'yev, O. A.; Dolgikh, V. A.; Lightfoot, P.; Ruck, Michael (August 2004). "Nd2(SeO3)2(SeO4)· 2H2O– a Mixed-Valence Compound containing Selenium in the Oxidation States+IV and+VI" (in de). Zeitschrift für anorganische und allgemeine Chemie 630 (10): 1395–1400. doi:10.1002/zaac.200400109. ISSN 0044-2313. https://onlinelibrary.wiley.com/doi/10.1002/zaac.200400109.
16. ↑ Morris, Russell E.; Wilkinson, Angus P.; Cheetham, Anthony K. (November 1992). "A novel mixed-valence selenium(IV)/selenium(VI) oxo compound: crystal structure determination and x-ray absorption near edge structure study of erbium selenite(IV) selenate(VI) hydrate, Er(SeO3)(SeO4)1/2•H2O" (in en). Inorganic Chemistry 31 (23): 4774–4777. doi:10.1021/ic00049a012. ISSN 0020-1669. https://pubs.acs.org/doi/abs/10.1021/ic00049a012.
17. ↑ Yankova, Rumyana; Genieva, Svetlana; Halachev, Nenko; Dimitrova, Ginka (February 2016). "Molecular structure, vibrational spectra, MEP, HOMO-LUMO and NBO analysis of Hf(SeO3)(SeO4)(H2O)4" (in en). Journal of Molecular Structure 1106: 82–88. doi:10.1016/j.molstruc.2015.10.091. Bibcode: 2016JMoSt1106...82Y. https://linkinghub.elsevier.com/retrieve/pii/S0022286015303914.
18. ↑ Wickleder, Mathias S.; Büchner, Oliver; Wickleder, Claudia; el Sheik, Sherif; Brunklaus, Gunther; Eckert, Hellmut (September 2004). "Au2(SeO3)2(SeO4): Synthesis and Characterization of a New Noncentrosymmetric Selenite−Selenate" (in en). Inorganic Chemistry 43 (19): 5860–5864. doi:10.1021/ic049270z. ISSN 0020-1669. PMID 15360234. https://pubs.acs.org/doi/10.1021/ic049270z.
19. ↑ Li, Peng-Fei; Hu, Chun-Li; Kong, Fang; Mao, Jiang-Gao (2022). "Hg 2 (SeO 3 )(SO 4 ): the first sulfate selenite with large birefringence explored from d 10 transition metal compounds" (in en). Materials Chemistry Frontiers 6 (23): 3567–3576. doi:10.1039/D2QM00773H. ISSN 2052-1537. https://xlink.rsc.org/?DOI=D2QM00773H.
20. ↑ Weil, Matthias; Kolitsch, Uwe (2002-04-15). "Hg3Se3O10, a mercury(II) compound with mixed-valence oxoselenium(IV/VI) anions". Acta Crystallographica Section C Crystal Structure Communications 58 (4): i47–i49. doi:10.1107/S0108270102001920. ISSN 0108-2701. PMID 11932512. Bibcode: 2002AcCrC..58I..47W. http://scripts.iucr.org/cgi-bin/paper?S0108270102001920.
21. ↑ Li, Peng-Fei; Hu, Chun-Li; Li, Bing-Xuan; Mao, Jiang-Gao; Kong, Fang (2024-02-16). "Hg3Se(SeO3)(SO4): A Mixed-Valent Selenium Compound with Mid-Infrared Transmittance Obtained by In Situ Reaction" (in en). Inorganic Chemistry 63 (9): 4011–4016. doi:10.1021/acs.inorgchem.4c00033. ISSN 0020-1669. PMID 38363859. https://pubs.acs.org/doi/10.1021/acs.inorgchem.4c00033.
22. ↑ Weil, Matthias; Shirkanlou, Mahdi (July 2015). "Hydrothermal Studies in the System Hg/Se/Te/O: The First Te IV /Se VI Oxocompounds Hg3SeTe2O10 and Hg3SeTe4O14, and the Mixed-valent Hg5Se2O8: Hydrothermal Studies in the System Hg/Se/Te/O" (in en). Zeitschrift für anorganische und allgemeine Chemie 641 (8–9): 1459–1466. doi:10.1002/zaac.201500171. https://onlinelibrary.wiley.com/doi/10.1002/zaac.201500171.
23. ↑ 23.0 23.1 Weil, Matthias (2004-10-01). "The crystal structures of Hg7Se3O13H2 and Hg8Se4O17H2 — two mixed-valent mercury oxoselenium compounds with a multifarious crystal chemistry" (in en). Zeitschrift für Kristallographie - Crystalline Materials 219 (10): 621–629. doi:10.1524/zkri.219.10.621.50817. ISSN 2196-7105. Bibcode: 2004ZK....219..621W. https://www.degruyter.com/document/doi/10.1524/zkri.219.10.621.50817/html.
24. ↑ 24.0 24.1 Wang, Xiao-Xue; Li, Xiao-Bao; Hu, Chun-Li; Kong, Fang; Mao, Jiang-Gao (December 2019). "Ag4Hg(SeO3)2(SeO4): a novel SHG material created in mixed valent selenium oxides by in situ synthesis" (in en). Science China Materials 62 (12): 1821–1830. doi:10.1007/s40843-019-1193-x. ISSN 2095-8226.
25. ↑ Effenberger, H. (January 1987). "Crystal structure and chemical formula of schmiederite, Pb2Cu2(OH)4(SeO3)(SeO4), with a comparison to linarite, PbCu(OH)2(SO4)" (in en). Mineralogy and Petrology 36 (1): 3–12. doi:10.1007/BF01164365. ISSN 0930-0708. Bibcode: 1987MinPe..36....3E. http://link.springer.com/10.1007/BF01164365.
26. ↑ Lee, Eun Pyo; Song, Seung Yoon; Lee, Dong Woo; Ok, Kang Min (2013-04-01). "New Bismuth Selenium Oxides: Syntheses, Structures, and Characterizations of Centrosymmetric Bi2(SeO3)2(SeO4) and Bi2(TeO3)2(SeO4) and Noncentrosymmetric Bi(SeO3)(HSeO3)" (in en). Inorganic Chemistry 52 (7): 4097–4103. doi:10.1021/ic4002384. ISSN 0020-1669. PMID 23506341. https://pubs.acs.org/doi/10.1021/ic4002384.
27. ↑ Sullens, Tyler A.; Almond, Philip M.; Byrd, Jessica A.; Beitz, James V.; Bray, Travis H.; Albrecht-Schmitt, Thomas E. (April 2006). "Extended networks, porous sheets, and chiral frameworks. Thorium materials containing mixed geometry anions: Structures and properties of Th(SeO3)(SeO4), Th(IO3)2(SeO4)(H2O)3·H2O, and Th(CrO4)(IO3)2" (in en). Journal of Solid State Chemistry 179 (4): 1192–1201. doi:10.1016/j.jssc.2006.01.017. Bibcode: 2006JSSCh.179.1192S. https://linkinghub.elsevier.com/retrieve/pii/S0022459606000211.
28. ↑ Krivovichev, S. V. (December 2009). "Crystal chemistry of selenates with mineral-like structures: VII. The structure of (H3O)[(UO2)(SeO4)(SeO2OH) and some structural features of selenite-selenates"] (in en). Geology of Ore Deposits 51 (7): 663–667. doi:10.1134/S1075701509070150. ISSN 1075-7015. Bibcode: 2009GeoOD..51..663K. http://link.springer.com/10.1134/S1075701509070150.
29. ↑ Krivovichev, S. V.; Tananaev, I. G.; Kalenberg, V.; Myasoedov, B. F. (2005). "Synthesis and crystal structure of the first uranyl selenite(IV)-selenate(VI), [C5H14N[(UO2)(SeO4)(SeO2OH)]"] (in Russian). Doklady Akademii Nauk - Rossijskaya Akademiya Nauk 403 (3): 349–352. ISSN 0869-5652. http://inis.iaea.org/Search/search.aspx?orig_q=RN:38076927.
30. ↑ Krivovichev, S. V.; Tananaev, I. G.; Kahlenberg, V.; Myasoedov, B. F. (May 2006). "Synthesis and crystal structure of a new uranyl selenite(IV)-selenate(VI), [C5H14N4[(UO2)3(SeO4)4(HSeO3)(H2O)](H2SeO3)(HSeO4)"] (in en). Radiochemistry 48 (3): 217–222. doi:10.1134/S1066362206030027. ISSN 1066-3622. Bibcode: 2006Radch..48..217K. http://link.springer.com/10.1134/S1066362206030027.
31. ↑ 31.0 31.1 Gurzhiy, Vladislav V.; Kovrugin, Vadim M.; Tyumentseva, Olga S.; Mikhaylenko, Pavel A.; Krivovichev, Sergey V.; Tananaev, Ivan G. (September 2015). "Topologically and geometrically flexible structural units in seven new organically templated uranyl selenates and selenite–selenates" (in en). Journal of Solid State Chemistry 229: 32–40. doi:10.1016/j.jssc.2015.04.040. Bibcode: 2015JSSCh.229...32G. https://linkinghub.elsevier.com/retrieve/pii/S0022459615001759.
32. ↑ Gurzhiy, V. V.; Krivovichev, S. V.; Burns, P. C.; Tananaev, I. G.; Myasoedov, B. F. (February 2010). "Supramolecular templates for the synthesis of new nanostructured uranyl compounds: Crystal structure of [NH3(CH2)9NH3[(UO2)(SeO4)(SeO2OH)](NO3)"] (in en). Radiochemistry 52 (1): 1–6. doi:10.1134/S1066362210010017. ISSN 1066-3622. Bibcode: 2010Radch..52....1G. http://link.springer.com/10.1134/S1066362210010017.
33. ↑ Wylie, E. M.; Burns, P. C. (2012-02-01). "Crystal Structures of Six New Uranyl Selenate and Selenite Compounds and Their Relationship with Uranyl Mineral Structures" (in en). The Canadian Mineralogist 50 (1): 147–157. doi:10.3749/canmin.50.1.147. ISSN 0008-4476. Bibcode: 2012CaMin..50..147W. http://www.canmin.org/cgi/doi/10.3749/canmin.50.1.147.

* v
* t
* e

Selenium compounds

Se(−II)|

* Ag2Se
* Al2Se3
* CaSe
* Se2−

Se(0,I)|

* Se3S5

Se(I)|

* Se2S6
* Se2Cl2
* C3H7NO2Se

Se(II)|

* SeS2

Se(IV)|

* SeCl4
* SeF4
* SeO2
* SeS2
* SeOBr2
* SeOCl2

Se(VI)|

* SeF6
* SeO3
* SeO2F2

Template:Selenites

0.00

(0 votes)

Original source: https://en.wikipedia.org/wiki/Selenate selenite. Read more

|

Retrieved from "https://handwiki.org/wiki/index.php?title=Chemistry:Selenate_selenite&oldid=4433965"
*[v]: View this template
*[t]: Discuss this template
*[e]: Edit this template